Zinc Coating on Aluminum-Alloy Substrate by
Syed Roohullah Jan1, Kareem Akhtar2, Naeem Khan3, Syed Nasratullah4, Zabiullah4, Farhan Faiz Durani4, Usman Awan4, Ahmad Ameen4.
Lecturer, Dept. of Mechanical Engineering, University of Engineering and Technology, Peshawar, KPK, Pakistan1 Asst. Professor, Dept. of Mechanical Engineering, University of Engineering and Technology, Peshawar,
Professor, Dept. of Mechanical Engineering, University of Engineering and Technology, Peshawar, KPK, Pakistan3 Students, Dept. of Mechanical Engineering, University of Engineering and Technology, Peshawar, KPK, Pakistan4 *Corresponding Author
ABSTRACT: Metallic coatings that are generated by conventional techniques encounter many problems. These coatings are affected by oxidation and contamination as the coating is developed by spraying melted material. To achieve rapid, economical and phase pure metallic coatings, cold spray technique is applied. This work consists of similar technique used for development of Zinc coatings on aluminum-alloy as base material. Pure coatings were achieved by using convergent-divergent nozzle. Composition of the zinc powder and the aluminum-alloy substrate were investigated prior to coatings. The particle size distribution of coated powder was also found. Zinc coatings were generated with help of designed cold spray facility. It was then characterized using scanning electron microscopy. The effect of coatings on substrate hardness was determined by micro vickers hardness test apparatus. The study revealed that using cold spray zinc coating on Aluminum-alloy substrate can be achieved at room temperature. Since all the particles are of range 1-50 microns, very thin layer but continuous (no gaps/voids) can be achieved. Such fine coating would be impossible using conventional methods of metal coatings. Coatings cross-sections show that good bonding was established. The hardness test reveals that surface strength increases due to deposition of metal particles.
KEYWORDS:Cold spray; Zinc powder; Aluminium Alloy; Solid state coating.
Presently the metallic coatings are developed by Thermal coating techniques. It has limited application due to melting the coating material, oxidation problems of coatings and non-applicability to the high temperature sensitive metals. Thermal coating techniques are also time consuming and uneconomical.
This study presents a new technique for development of metallic coatings, known as cold spray. In this process the metals, to be coated, are taken in powder form. Coating is made at room temperature by accelerating metallic powder to supersonic speed using a convergent-divergent nozzle. The velocity limit for various metals depends on its mechanical properties and is different for each one. These high speed particles when strike the base material, it undergoes plastic deformation due to abrupt change in particles-momentum. It lead to shear deformation of particles and results in a continuous coating on base material [1, 2].
Contrary if the powder particles are injected in the diverging section of convergent-divergent nozzle, it is called Low pressure cold spray (LPCS). In this process because of low pressure expending gases the pressure in powder chamber is comparatively low than the HPCS . Except from powder injection method both has same operating conditions. The HPCS results in high coating efficiency than LPCS while nozzle life is longer for LPCS. 
II. WHY ZINC IS COATED ON ALUMINIUM
The most plentiful element on the earth crust is Aluminum and it comprises almost 8.23 % of it. It is well known for its light weight and high ratio of strength to weight. Also in comparison to steel it has one-third of its stiffness. One major problem that aluminum undergoes is its surface oxidation when exposed to environment. It develops a layer of aluminum oxide (Al2O3) on its surface. This oxide layer decreases oxidation rate but it is electrical insulator and has
brittle nature . Aluminum alloys on other hand are more prone to surface oxidation process. There are three Existent techniques to prevent this surface oxidation. It consist of “alclading” , secondly the “chromate conversion coating”  and the third one is “anodizing”  .
The metal zinc contrary to aluminum possesses corrosion resistance nature and has fair electrical conductivity . It is, therefore, evident that coating aluminum with zinc can improve its corrosion resistance with minimum effect on its electrical properties.
III. COLD SPRAY PARAMETERS AND BONDING MECHANISM
The cold spray parameters are particle size and shape; stagnation pressure and temperature; nozzle design its standoff distance and spray angle; and carrier gas. The carrier gas for particle is selected as Helium, Nitrogen, air or mixture of Helium and air. Helium gas causes highest particles velocity followed by nitrogen and the air [11, 12]. The gas pressure is maintained higher in powder chamber than in nozzle at point of ejection for smooth flow of powder. Velocity of particles at exit of nozzle depends on the gas velocity in nozzle and its expansion in divergent section of nozzle . When particles at high speed, greater than a critical value, collide with the substrate, a high pressure field is generated at point of contact and it then proceeds in particle and substrate. The stress generated is greater than the yield stress and it leads to a phenomenon known as ‘adiabatic shear instability’. It causes plastic deformation of particles along the shear plane and the material accelerates laterally producing localized shear straining. The oxide layer is partially removed and pure metallic interaction occurs . Flow stresses are, therefore, breakdown due to discontinuous leaps in strain and localize temperature [15-20].
In this study development of zinc coating on aluminum 6005-alloy as substrate will be discussed using HPCS technique. It is only possible if zinc particles are accelerated above its critical velocity that is 350 m s-1 . Elemental composition of zinc powder and substrate was found by Energy dispersive X-ray spectroscopy (EDX). Particle size range was investigated by particles size analyzer (Multisizer-3). Coating was performed with self made cold spray facility using convergent-divergent nozzle. Operating pressure of 10 bars was achieved by water cooled two stage air compressors. The coatings were characterized by using scanning electron microscope (SEM). The micro-hardness test of coating was performed to find effect of coating on surface hardness of base material.
Fig. 1: Particle size study by Multisizer.3.
Particle size distribution curve of zinc is shown in above fig and particles ranges from 1 micron to 20 microns. On x-axis particle diameter is mentioned while on y-x-axis relative quantity in number is shown. Most of the particles was in range of 1-10 microns.
Aluminium substrate surface composition
Aluminum 6005-alloy with gauge thickness of “1 mm” was used as a substrate for coating. The elemental composition of as-received substrate was found out by EDX.
Fig. 2: EDX compositional peaks of Aluminum substrate.
Table 1: Percent weight composition.
In above table relative weight percentages of various compositional elements are also presented. All elements add up to make a total of 100% weight percent.
Zn powder composition investigation
Elemental composition of Zinc powder was also investigated by EDX. The obtained result is presented in figure 3, which shows all the Elemental peaks for zinc carbon and oxygen.
Fig. 3: EDX compositional peaks of Zn-powder.
On x-axis of above figure, is the intensity while on y-axis is amount of energy released due to electron transitions from high energy shell. Both high energy peaks with low intensity for high shell transition electrons and low energy with high intensity for low shell transition electron is shown.
Table 2: Percent Weight composition.
traces of Carbon and oxygen.
V. EXPERIMENTAL PROCEDURE OF COLD SPRAY
Cold spraying was performed on cold spray facility. A two stage Air-compressor was used to build the required pressure of 10 bars in a pressurize cylinder. A self made converging-diverging nozzle was used to generate Zn-coatings on aluminum substrate. The air-operated supersonic nozzle used for coating is shown in figure 4.
Fig. 4: Cold spray nozzle.
The above nozzle was having a converging part of length of 40 mm and diverging part of length of 100 mm with powder feeder attached to nozzle before the converging part. The powder chamber was pressurized a little above 10 bars to avoid back flow of powder and attached to the nozzle at an angle of 450. The powder was having gravitational effect and was also pressed by high pressure air. This causes powder to passes through a 2 mm hole provided at the base and was injected radial into the nozzle before the converging part. The design parameters of nozzle are shown in table 3.
Before coating the substrate was rough polished to get rid of all surface impurities. The coating was made by clamping the substrate in a cold spray chamber at 90o angle to the nozzle. During coating the nozzle was given movement in transverse direction at 50 mm s-1 and was kept 40 mm away from substrate. The nozzle was given several repetitions to get thick coating during spray process. After coating the samples were shear-cut from the substrate to carry the coating characterization. Surface hardness before coating and after coating was also checked.
VI.EXPERIMENTAL RESULTS AND DISCUSSION
Coating surface characteristics
Coating characterization was done by sectioning proper size samples from coated surface. SEM was used to study coating surface. Coating Image at magnification of 500X, 1000X and at 20kv are shown in figure 5. It shows voids-free and continuous zinc-coatings. The white region on black background is because reflection of electrons from different deep and shallow coating surface.
Fig. 5: Scanning Electron Microscope (SEM) images of coated surface at different magnification at 500X.
Coating cross-section characteristics
Cross-sections of the coating at magnification of 750 X as shown in figure 7.
Fig. 7: Scanning electron microscope (SEM) image of coating cross-section at magnification of 750 X.
Above figure represents the continuous layers of coating of Zn on aluminium substrate. During coating different particles collide and hence deposit on each other forming continuous layers. It also illustrates that particles are well bonded with the substrate.
Hardness test was performed by applying 100g load for 15sec on substrate before coating and then in-coated form. The micro-hardness of substrate was 50.5Hv0.1/15 and after coating it increased to 94.71Hv0.1/15. The increase in hardness is because of cold working of substrate by zinc particles. The resulted hardness is due to combined interaction of zinc-powder and aluminium substrate.
In cold spray process, continuous coating was achieved and good bonding occurred between coating and interface. Bonding between various layers of coating was also good and hence thick coatings can be generated for different engineering applications. Also as a result of cold working process, hardness of substrate was increased.
Critical velocity of Zinc is achieved with designed nozzle as deposition is only possible if velocity of micro-particles is greater than critical velocity.
VIII.FUTURE WORK AND MODIFICATIONS
Coating quality can be enhanced by controlling leakage problem from powder chamber and devising proper mechanism of powder injection. By installation of pressure gauge at inlet of the nozzle the pressure losses in pipe can be counteract. It facilitates to achieve higher velocity of particles. Cold spray chamber can also be manufactured for ensuring health and safety.
. Papyrin, A., Kosarev, V., Klinkov, S., Alkhimov, A., and Fomin, V., Cold Spay Technology,2007.
. Kosarve, V.F., Klinkov, S. V., Alkhimov, A. P., and Papyrin, A. N., On Some Aspects of Gas Dynamics of the Cold Spray Process Journal of Thermal Spray Technology, 12, p. 265–281, 2001.
. Fauchais, P.a.M., G., Thermal and cold spray: recent developments. Journal of Thermal Spray Technology, 384, p. 1-59, 2008. . Makeitfrom.com. Material Properties Data: Alumina (Aluminum Oxide).
. Moran., J.S.a.J., Corrosion Resistance of Aluminum Alloys. Corrosion: Fundamentals, Testing and Protection. ASM Handbook. ASM, 2003.
. K.H.J.C. Buschow, Robert W.; Flemings, Merton C.; Ilschner, Bernhard; Kramer, Edward J.; Mahajan, Subhash Editor.Encyclopedia of Material - Science and Technology ,Elsevier: Oxford, UK, p. 1265, 2001.
. Sheasby, P.G.P., R. , The Surface Treatment and Finishing of Aluminum and its Alloys., ed. s. ed.), Materials Park, Ohio & Stevenage, UK: ASM International & Finishing Publications, 2001.
. Taylor & Francis Group. Florida: Boca Raton., Handbook of Chemistry and Physics (87th ed.) ed. Vol. CRC Press, 2006.
. R.E. Blose, T.J.R., A.J. Mayer, D.E. Beatty, A.N. Papyrin, Advancing the Science and Applying the Technology. Thermal Spray, 2003. . T.H. Van Steenkiste, J.R.S., R.E. Teets, Surf. Coat. Tech., p. 237, 2002.
. Singh, H., Sidhu, T. S., and Kalsi, S. B. S., Cold spray technology: future of coating deposition processes, 22, p. 69–84, 2012. . M. Grujicic, C.L.Z., W.S. DeRosset, D. Helfritch, Mater. Design, 25, p. 681, 2004.
. Klinkov, S.V., Kosarev, V. F., and Rein, M., Cold spray deposition: Significance of particle impact phenomena. Aerospace Science and Technology. Vol. 9. 2005.
. Li, W.Y., Zhang, C., Li, C. J., and Liao, H., Modeling Aspects of High Velocity Impact of Particles in Cold Spraying by Explicit Finite Element Analysis. Journal of Thermal Spray Technology.
. Assadi, H., Gartner, F., Stoltenhoff, T., and Kreye, H., Bonding mechanism in cold gas spraying. Acta Materialia. Vol. 51,4379–4394, 2003.
. Bae, G., Xiong, Y., Kumar, S., Kang, K., and Lee, C., General aspects of interface bonding in kinetic sprayed coatings,”. Acta Materialia Vol. 56,4858–4868, 2008
. Spencer, K., Luzin, V., and Zhang, M., Structure and Properties of Cold Spray Coatings, in Materials Science Forum, p. 4379-4394, 2010. . Saleh, M., Luzin, V., and Spencer, K., Analysis of the residual stress and bonding mechanism in the cold spray technique using
experimental and numerical methods.